Recommended Construction Guidelines
Full Depth Reclamation (FDR)
Using Bituminous Stabilization
It is not intended or recommended that these guidelines be used verbatim within a specification.
Owner Agencies should use them to help establish their particular project specification. Owner
Agencies should understand that all geographical areas and pavement rehabilitation/preservation
projects are unique and the availability of materials and equipment may vary as well. ARRA assumes
no liability for utilization of these guidelines by any individual or entity. Contact ARRA for answers to
questions and for a list of ARRA member Contractors and Suppliers.
Asphalt Recycling & Reclaiming Association
800 Roosevelt Road, Building C-312
Glen Ellyn, IL 60137
Full Depth Reclamation (FDR) shall consist of pulverizing (reclaiming) the existing flexible pavement
and underlying materials (base and/or subgrade materials) to the length, depth and width as
specified or as shown on the plans, blending with a bituminous stabilizing agent (either foamed
asphalt, also known as expanded asphalt, or emulsified asphalt), water and other additives (cement,
lime, lime kiln dust, fly ash or corrective aggregate) as required by the mix design, to produce a
flexible, bituminous stabilized base. This material shall then be shaped, compacted, cured and
protected in accordance with the plans and specifications.
2. Treatment Thickness
The existing flexible pavement, base and/or subgrade material shall be pulverized to a total depth of
____ inches (mm). The pulverized section shall then be re-graded, with excess material hauled away
as necessary, so as to allow for the net placement of ____ inches of new pavement material.
Bituminous stabilizing agent, water, additives, and/or corrective aggregate shall be added and
blended to a total depth of ____ inches (mm) in accordance with the plans and specifications.
User Note: FDR treatment thicknesses may vary between 4 and 12 inches (100 - 300 mm) per lift and
should be dependent on structural capacity requirements and project-specific criteria such as original
asphalt pavement thickness and design life. Selecting the right FDR application for a particular project
should be based on the judgment of those involved in the design process of the project after
consideration of several key factors including: project location, existing roadway conditions, depth of
current pavement layers, failure depths, reason for current failure (i.e. lack of maintenance, age,
insufficient depth, lack of adequate drainage, etc.), traffic volume, available materials, and project
3. Preconstruction Personnel Training
Personnel involved with the construction of FDR from both the Contractor and Owner Agency shall
have successfully completed Preconstruction Personnel Training (PPT) to ensure that proper quality
procedures are followed to construct high quality FDR stabilized base. The PPT shall be conducted at
a location convenient for both the Contractor and the Owner Agency. The PPT shall be completed not
more than ___ days, not including Saturdays, Sundays or holidays, prior to the start of FDR
operations. The training shall be held during normal working hours. In lieu of this training, proof may
be provided showing successful experience has been obtained by the individuals performing the
work for the materials and construction techniques to be used in the FDR construction.
The PPT trainer shall be provided by the ___________ (Contractor or Owner Agency). The PPT
trainer shall be experienced in construction methods, materials, and test methods associated with
construction of FDR projects. The Contractor and Owner Agency shall mutually agree to the course
instructor, course content and training site.
User Note: PPT is optional to the agency. PPT should be conducted for agencies and Contractors new
to FDR. It is recommended that the PPT takes place within 5 days from the start of the FDR so that it
is current and allows some time to address any issues that may be raised during the training.
FDR shall consist of a homogeneous blend of reclaimed asphalt pavement (RAP), base material
and/or subgrade materials, bituminous stabilizing agent (either foamed asphalt or emulsified
asphalt), water, and other chemical additives and corrective aggregate as necessary. The actual
materials utilized and their respective usage rates are dependent on the mix design and project
4.1 Reclaimed Asphalt Pavement and Underlying Material
RAP and underlying material shall consist of the existing asphalt material, existing base course
material and/or subgrade material. The underlying materials shall be free of roots, sod, topsoil,
weeds, wood or any material deleterious to its reaction with the bituminous stabilizing agent. The
gradation of the processed (pulverized) material shall meet the requirements of Table 1.
Note: For asphalt emulsion, the recommended range on the No. 200 sieve is 2-15% and 5-20% for foamed
asphalt. Although not specified, the optimal range for percent passing the No. 4 (4.75 mm) sieve is 35 to 60
Rubberized crack filler, pavement markers, loop wires, thermoplastic markers, paving fabric and
other similar materials shall be removed as observed from the roadway during the reclaiming
process. Residual materials that cannot be completely removed from the reclaimed material may be
incorporated into the FDR mixture if the Contractor can demonstrate that those added materials will
not adversely affect performance. Any such materials retained in the mixture shall be appropriately
sized and blended so as to not adversely affect the appearance or strength of the FDR stabilized base.
4.2 Bituminous Stabilizing Agent
Bituminous stabilizing agent shall consist of either asphalt binder used to produce foamed asphalt or
emulsified asphalt. Unless indicated elsewhere within the plans, project specifications, or an Owner
Agency supplied mix design, the Contractor shall select the type and grade of stabilizing agent
4.2.1 Asphalt Binder for Foamed Asphalt
Asphalt binder used to produce foamed bituminous stabilization shall be selected according to local
temperature standards and specifications and to ensure that optimum foaming characteristics are
met in the field. Polymer modified asphalt binders shall not be used. The asphalt binder shall not be
heated above a temperature of 375° F (190° C). Asphalt binder provided to the job shall not have
additives or properties which could inhibit the ability to produce asphalt foam with a minimum
expansion ratio of ____, and a half-life of not less than ____ seconds. The application rate shall be
determined by the mix design.
User Note: The expansion ratio is defined as the volume of foamed asphalt to residual unfoamed
asphalt. The half-life is defined as the time for the foamed asphalt to lose half of its expanded
volume. Typically, the asphalt binder must exceed 320° F (160° C) to achieve optimum foaming
Table 1 – GRADATION OF PROCESSED
Sieve Size Percent
3 in. (75 mm) 100
2 in. (50 mm) 95-100
No. 200 (0.075 mm) 2-20
characteristics; however, this temperature may vary depending on the type of asphalt binder used.
Typical expansion ratios should be a minimum of 8 and the half-life should be a minimum of 6.
4.2.2 Emulsified Asphalt
Emulsified asphalt shall be selected to meet local standards and specifications and to achieve
appropriate mixing with the pulverized material. A mixing grade emulsion shall be used. Polymer
modification may also be used. The actual emulsion type and applicable rate shall be determined
by the mix design.
4.3 Corrective Aggregate
Corrective aggregate may be required to supplement the existing material gradation and to meet
performance requirements of the mix design. Corrective aggregate may consist of crushed rock, RAP,
crushed concrete or other types of aggregate approved by the Owner Agency. The corrective
aggregate gradation may vary according to its size and distribution, depending on the desired effect
to the FDR stabilized base. When required by the mix design, corrective aggregate shall meet the
requirements of Table 2.
TABLE 2 – CORRECTIVE AGGREGATE
Tests Method Limit
Los Angeles Abrasion Value, % loss AASHTO T 96
Sand Equivalent,% AASHTO T 176
Washed Gradation AASHTO T 11 & T 27
ASTM C117 & C136
4.4 Chemical Additives
If required by the mix design, bituminous stabilizing agents may be supplemented with small
quantities of the following chemical additives to enhance mixture properties and facilitate
Cement (portland or blended hydraulic), in either dry or slurry form, may be added to the reclaimed
mixture as determined by the mix design. Slurry made from cement shall contain a minimum of 30%
dry solids content. Cement used for full depth reclamation shall comply with the latest specifications
for hydraulic cement (AASHTO M 85, AASHTO M 240 or ASTM C150, ASTM C595. The ratio of residual
asphalt in the bituminous stabilizing agent to dry cement shall be at least 3: